- Polyoxymethylene plastic
Polyoxymethylene (POM), in the USA also commonly known under
DuPont's brand name Delrin, is an engineering plastic, a polymerwith the chemical formula -(-O-CH2-)n-. It is often marketed and used as a metalsubstitute. Delrin is a lightweight, low-friction, and wear-resistant thermoplasticwith good physical and processing properties and capable of operating in temperatures in excess of 90 degrees celsius(approximately 200 degrees fahrenheit). According to the material safety data sheetfrom DuPont, the material has a slight odor of formaldehyde. [ [http://eiecomprod.shopforplastics.com/Ensinger/msds/delrin.html Dupont MSDS for Delrin] ]
It is also known as polyacetal, acetal resin, polytrioxane, polyformaldehyde, and
paraformaldehyde(the latter term is usually restricted to the short-chained polymer). Polyacetals are sold under the trade names Delrin, Kepital, Celcon, Hostaform, Iupital [Citation | title = Iupital | url = http://www.m-ep.co.jp/mep-en/products/iupital/ | accessdate = 25-05-2008.] and Ultraform [ [http://www.plasticsportal.net/wa/plasticsEU~en_GB/portal/show/content/products/engineering_plastics/ultraform BASF Ultraform product information] ] , the last five being copolymers.
Delrin was first synthesized by DuPont's research chemists around 1952. The company filed for patent protection of the material in 1956 and completed construction of a plant to produce the material at
Parkersburg, West Virginiain 1960. Another form of the polymer was developed in Europe.
The polymer shares common characteristics with other synthetic polymers such as low density (1.4 - 1.5 g/cm3), and ease of moulding when the
molecular weightis low enough. It is a semi-crystalline polymer (75-85% crystalline) with a melting point of 175 °C as a homopolymer. A copolymerversion has slightly lower melting point of 163 °C. It is a tough material with a very low coefficient of friction. However, it is suceptible to polymer degradationcatalysed by acids, which is why both polymer types are stabilised. In the case of the homopolymer, it has chain end groups which resist depolymerization. With the copolymer, the second unit is a cyclic etherwhich resist chain cleavage. It is also sensitive to oxidation, and an anti-oxidantis normally added to moulding grades of the material.
To make polyoxymethylene
homopolymer, anhydrousformaldehyde must be generated. The principal method is by reaction of the aqueous formaldehyde with an alcohol to create a hemiformal, dehydration of the hemiformal/water mixture (either by extraction or vacuum distillation) and release of the formaldehyde by heating the hemiformal. The formaldehyde is then polymerized by anionic catalysisand the resulting polymer stabilized by reaction with acetic anhydride.
To make polyoxymethylene copolymer, formaldehyde is generally converted to trioxane. This is done by
acid catalysis(either sulfuric acidor acidic ion exchange resins) and concurrent removal of the trioxane by distillation or extraction. The trioxane is then dried to remove all water and other active hydrogen containing impurities.
The co-monomer is typically
dioxolanebut ethylene oxidecan also be used. Dioxolane is formed by reaction of ethylene glycolwith a formaldehyde source (trioxane or concentrated aqueous formaldehyde) over an acid catalyst. Other diols can also be used.
Trioxane and Dioxolane are polymerized using an acid catalyst, often boron trifluoride etherate, BF3·OEt2. The polymerization can take place in a non-polar
solvent(in which case the polymer forms as a slurry) or in the melt (e.g. an extruder). After polymerization, the acidic catalyst must be deactivated and the polymer stabilized by heat.
Stable polymer is melt compounded, adding thermal and oxidative stabilizers and optionally lubricants and miscellaneous fillers.
Food and Drug Administrationhas approved Delrin for use in the food industry. Delrin was used by Mattelfrom 1968 to 1972 to produce the low-friction wheel bearings found on redline Hot Wheels. Delrin is made from acetalhomopolymer resin, and, when extruded into large basic shapes (i.e., sheets, rods, and tubes), tends to be subject to porosity problems. These porosity problems can make the product less reliable in certain applications. Acetal copolymer (Acetron GP) is often used as a replacement for Delrin (acetal homopolymer) when porosity risk is a factor in material selection.
It is also used in
yo-yos such as the Silk by Alchemy yoyos, Lyn Fury by YoYoJam, and the Milk by Born Crucial. Delrin's lubricity (when machined on a lathe) leads to a yo-yo with significantly less friction.
It is also used extensively in
paintball markers, where it is used to make bolts, pump handles and many other parts. Its low cost, adequate strength, light weight, and self-lubricating properties make it ideal for markers. The other material commonly-used for markers, Nylatron, while slightly lighter, is more prone to swelling. A swelled part can make the mechanism impossible to operate and sometimes even damages the marker. Nylon-based products such as Nylatron have better wear-resistance than Delrin, but do not have good moisture-resistance, and are therefore not suitable to high-humidity or underwater applications.
Delrin's resistance to liquids and low coefficient of friction have also made it useful as a bearing-replacement in
casters and wheels, to be selected in cases where corrosive environments make a traditional roller or ball bearingimpractical.
Delrin has also recently found use in the manufacturing of
Irish flutes (traditionally made of wood), tin whistles (traditionally made of metal), and bagpipes(traditionally made of wood). Delrin flutes sound similar or identical to wooden flutes, but have none of the shrinkage or cracking issues usually associated with wooden instruments in hot, cold, or dry environments. Builders such as Des Seery, Michael Cronnolly of M&E Flutes, Tony Dixon, and Rob Forbes all build Delrin flutes.
Delrin has become an increasingly popular material in the fabrication of
guitar picks. It has excellent durability; it is much more resistant to wear than nylonat the point of string contact, especially on round-wound strings. Delrin does not crack or break like celluloidor polyvinyl chloride(PVC), provides a solid, slip-free grip, and develops a "memory" over time; that is, it gradually develops a slight curvature that conforms to the user's grip.
Delrin is also much treasured by many makers and players of
harpsichords, being used for the plectra, which pluck the strings when a key is pressed. Delrin has been found to provide a tonal quality very similar to that of the bird-quill used in the heyday of the instrument, while being far more durable and consistent.
Delrin has also been used for many years by a number of cutlery manufacturers to make knife handles, especially for jacknives.
Delrin is used to make the combination wheels in most high-security safe locks. Using delrin in the wheels makes the lock resistant to decoding by X-raying because of delrin's low density. However, neutron bombardment techniques may still be used to decode delrin combination wheels. Delrin also increases the lock's resistance to wear.
It is also used to make frame sliders and knee pucks for motorcycle riders/racers, as well as for slide gloves used when
Delrin is gaining popularity for the manufacture of diving equipment, due to its light weight and its low porosity to gas under pressure. Some other plastics can absorb gas under pressure, and swell or deform.
Delrin has been used increasingly to create body-piercing jewelry, especially tunnels or plugs for use in stretched holes. While viewed by many as relatively safe for daily wear, the safety of this practice is still hotly debated within the piercing community.
Delrin is also being commonly used as a substitute for horn in the koiguchi on modern-made Japanese swords.
Two companies that made watthour meters also used Delrin components in their cyclometer-type registers for a while. However, Delrin has an unfortunate tendency to deteriorate when exposed to UV (from sunlight) for long periods of time - leading to performance issues in the register and a costly situation for the manufacturers.
Supplied in granulated form, POM can be formed into the desired shape by applying heat and pressure. The two most common forming methods employed are
injection moldingand extrusion. Rotational and blow moldingare also possible.
Typical applications for injection-molded POM include high performance engineering components (e.g. gear wheels, ski bindings, fasteners, lock systems) and the material is widely used in the automotive and consumer electronics industry. There are special grades that offer higher mechanical toughness, stiffness or low friction/ wear properties.
POM is commonly extruded as continuous lengths of round or rectangular section. These sections can be cut to length and sold as bar or sheet stock for machining.
It is commonly used by car manufacturers for many components of automobiles.
When supplied as extruded bar or sheet, Delrin may be machined using traditional methods such as turning, milling, drilling etc. These techniques are best employed where production economics do not merit the expense of melt processing. The material is free-cutting, but does require sharp tools with a high clearance angle. The use of soluble cutting lubricant is not necessary, but is recommended.
Because the material lacks the rigidity of most metals, care should be taken to use light clamping forces and sufficient support for the workpiece.
Machined Delrin can be dimensionally unstable, especially with parts that have large variations in wall thicknesses. It is recommended that such features are ‘designed-out’ e.g. by adding fillets or strengthening ribs. Annealing of pre-machined parts before final finishing is an alternative. A rule-of-thumb is that in general, small components machined in Delrin suffer from less warping.
Acetal polymers are typically very difficult to bond. Special processes and treatments have been developed to improve bonding of acetal. Typically these processes involve surface etching, flame treatment or mechanical abrasion. Typical etching processes involve
chromic acidat elevated temperatures. DuPont has a patented process for treating acetal homopolymer called satinizing which creates anchor points on the surface, giving an adhesive something to grab. There are also processes involving oxygen plasma and corona discharge [cite book
last = Snogren |first = R. C. |year = 1974 |title = Handbook of Surface Preparation |publisher = Palmerton Publishing Co. |location =New York] .
Once the surface is prepared, a number of adhesives can be used for bonding. These include epoxies,
polyurethanes, and cyanoacrylates. Epoxies have shown 150-500 psi shear strength on mechanically abraded surfaces and 500-1000 psi on chemically treated surfaces. Cyanoacrylates are useful for bonding to metal, leather, rubber and other plastics.
Solvent welding is typically unsuccessful on acetal polymers, due to the excellent solvent resistance of acetal. Thermal welding through various methods has been used successfully on both homopolymer and copolymer.
Acetal resins are sensitive to acid
hydrolysisand oxidationby such agents as chlorine, for example. Thus low levels of chlorine in potable water supplies can cause stress corrosion crackingto develop, a problem which has been experienced in both the USA and Europe in domestic and commercial water supply systems.
* [http://heritage.dupont.com/floater/fl_delrin/floater.shtml DuPont overview of Delrin]
* [http://www.machinedesign.com/BDE/materials/bdemat2/bdemat2_3.html General acetal resins overview]
Wikimedia Foundation. 2010.
Look at other dictionaries:
Paraformaldehyde — Chembox new ImageFile = Paraformaldehyd.svg ImageSize = 150px IUPACName = Polyoxymethylene OtherNames = Section1 = Chembox Identifiers CASNo = 30525 89 4 PubChem = 24898648 SMILES = Section2 = Chembox Properties Formula = (CH2O)n (n = 8 100)… … Wikipedia
1,3,5-Trioxane — Trioxin redirects here. For the fictitious chemical, see Return of the Living Dead (film series). 1,3,5 Trioxane IUPAC name … Wikipedia
Acetal — For the plastic, see Polyoxymethylene plastic. Not to be confused with Acetyl. Structure of a generic acetal … Wikipedia
Acetyl — In organic chemistry, acetyl (ethanoyl), is a functional group, the acyl of acetic acid, with chemical formula COCH3. It is sometimes abbreviated as Ac (not to be confused with the element actinium). The acetyl radical contains a methyl group… … Wikipedia
Formaldehyde releaser — A formaldehyde releaser is a chemical compound that slowly releases formaldehyde. Antimicrobials Formaldehyde releasers are often used an antimicrobial preservative in cosmetics. Examples include:* Quaternium 15 * Imidazolidinyl urea (Germall… … Wikipedia
Drucker Prager yield criterion — Continuum mechanics … Wikipedia
industrial polymers, major — Introduction chemical compounds used in the manufacture of synthetic industrial materials. In the commercial production of plastics, elastomers, man made fibres, adhesives, and surface coatings, a tremendous variety of polymers are… … Universalium
Polystyrene — For other uses, see Polystyrene (disambiguation). Expanded polystyrene packaging … Wikipedia
Cross-linked polyethylene — PEX redirects here. For other uses, see Pex (disambiguation). Cross linked polyethylene, commonly abbreviated PEX or XLPE, is a form of polyethylene with cross links. It is formed into tubing, and is used predominantly in hydronic radiant heating … Wikipedia
Resin identification code — Sorted household plastic waiting to be hauled away for reprocessing … Wikipedia